Digitized  by  the  Internet  Archive 
in  2016  with  funding  from 
Getty  Research  Institute 


https://archive.org/details/immedialcoloursoOOcass 


MANUFACTURE  LYONNAISE  DE  MATIERES  COLORANTES,  LYONS. 


Works  “La  Mouche”. 


RUSSIAN  ANILINE  COLOUR  WORKS  LEOPOLD  CASSELLA  & Co.,  RIGA. 


Works  at  Riga. 


LEOPOLD  CASSELLA  & C°-,  G.  m.  b.  H„  FRANKFORT 


Works  at  Mainkur  near  Frankfort 


IMMEDIAL  COLOURS  ON  PIECE-GOODS 


CASSELLA  COLOR  COMPANY 


182  and  184  FRONT  STREET 


NEW  YORK 


BOSTON:  39  Oliver  sjp^et,  , 

PHILADELPHIA:  12tf  and  128' SOUTH  ERO NT^REET 
PROVIDENCE:  64  exchange  place 
ATLANTA:  47  north  pryor  street 
MONTREAL:  Canada:  59  william  street. 


No.  3018. 


IMMEDIAL  COLOURS  ON  PIECE-GOODS 


The  Immedial  Colours  may  be  dyed 

a)  in  the  Jigger, 

b)  in  the  Padding  Machine, 

c)  in  the  Continuous  Machine. 

The  apparatus  must  not  contain  any  copper  or  brass  parts. 


DYEING  IN  THE  JIGGER. 

This  is  the  method  most  generally  employed.  The  so-called  “Immedial 
Jigger"  as  supplied  by  all  makers  of  textile  machinery*  is  used;  its  con- 
struction is  the  same  as  that  of  the  ordinary  jigger,  except  that  it  is 
provided  with  squeezing  rollers;  the  latter  may  be  attached  to  any  ordinary 
jigger  as  shown  in  the  following  sketch  (Fig.  1). 


Fig.  1. 


The  narrow  ends  (a)  of  the  jigger  are  fitted  with  two  bearings  (c)  which 
carry  a shaft  (d).  To  each  end  of  the  shaft,  right  and  left,  a lever  (e)  is  immov- 
ably affixed  by  means  of  a rabbet  and  wedge  carrying  the  squeezing  roller  (b)m 
The  levers  (e)  extend  beyond  the  roller  bearing  through  the  arms  (f),  which  may 
be  weighted  with  the  weights  (g).  When  not  in  actual  use,  the  whole  arrangement 
is  thrown  back  into  the  position  shown  by  the  dotted  lines,  and  is  there  arrested 
by  means  of  a bolt  which  passes  through  an  eye  in  arm  (h).  The  sprinkler  (i)  is 
fixed  as  shown  in  Fig.  3. 


* Jiggers  as  built  by  various  machine-makers  are  illustrated  in  our  book  “Blue 
Immedial  Colours”  (No.  2823). 


1 


During  the  dyeing  operation,  the  squeezing  rollers  are  turned  out 
of  use  over  the  middle  of  the  jigger,  the  dyeing  being  carried  out  as 
customary;  only  during  the  last  passage  is  the  squeezing  roller  applied, 
the  goods  passing  between  the  rollers,  and  then,  without  rolling  up,  straight 
into  the  rinsing  bath. 

For  the  dyeing  of  Immedial  Indone  and  Immedial  Indogene  it  has 
been  found  an  advantage  to  run  the  goods,  between  the  dyeing  and 
rinsing,  over  several  guiding  rollers  through  the  air  for  oxidising  purposes,  as 
shown  in  Fig.  2. 


'a"  Fig.  2.  ’3L 


In  Fig.  2 the  squeezing  rollers  are  pressed  down  by  screw  pressure  regulated 
by  the  wheel  ( c )\  in  Fig.  1 this  is  done  by  lever  pressure.  In  Fig.  2,  (d)  Indicates 
the  guiding  rollers  for  the  oxidation  and  (e)  the  sprinkler. 

In  Fig.  1 and  2,  ”a”  is  in  both  cases  the  dye-jigger;  jigger  ”b”  is  for 


As  Fig.  3 shows,  the  sprinkling-pipe  is  adjusted  in  the  rinsing  jigger  in  such  a 
manner  that  the  goods  are  given  a lively  sprinkling  on  both  sides  previous  to  the 
squeezing  off. 


2 


The  dyebaths  are  charged  with  sodium  sulphide  and  salt  in  accord- 
ance with  the  particulars  given  in  our  “Manual  of  Dyeing",  Vol.  I.  pages 
16 — 22.  except  that  for  small  bales  the  starting  baths  are  charged  with 
a little  more  dyestuff,  for  large  bales  on  the  other  hand  with  a little  less 
dyestuff  than  there  indicated. 

The  goods  to  be  dyed,  after  being  thoroughly  freed  from  size, 
should  be  beamed  evenly,  care  being  taken  also  during  the  dyeing  that 
the  goods  are  rolled  up  evenly. 

The  dyeing  is  effected  by  means  of  6 to  8 passages  in  a warm  or 
boiling  bath.  After  the  dyeing,  the  goods  are  squeezed  off  well,  and 
rinsed,  either  immediately  or  after  an  oxidation  in  the  air. 

Immedial  Blue  before  steaming  or  smothering  is  merely  squeezed 
off,  and  not  rinsed. 

The  following  are  a few  examples: 


Black  produced  with  Immedial  Black. 


10  pieces  mercerised  satteen 

Immedial  Black  NNG  cone. 
Sodium  sulphide  crystals 
Soda  ash 

Common  salt  or  desiccated 
Glauber’s  salt 


160  lbs  weight  in  goods  30  gallons  liquor 


Starting  bath: 
16  lbs  6 oz 
16  lbs  6 
V/2  lbs 


oz 


Additions  for  subsequent  lots: 
10  lbs  6 oz 
10  lbs  6 oz 
11/2-3  oz 


6 lbs 


1 lb 


The  goods  are  given  6 to  8 passages  at  boiling  temperature.  After 
squeezing  off,  they  are  rinsed  until  the  wash  water  is  perfectly  clear. 
To  the  last  rinsing  bath  5-8  oz  acetate  or  formate  of  soda  per  10  gallons 
water  are  added,  whereupon  the  goods  are  dried  without  rinsing  again. 


Blue  produced  with  Immedial  Direct  Blue  or  Immedial  New  Blue  G cone. 


5 pieces  moleskin  300  lbs  weight  in  goods  40  gallons  liquor 


Immedial  Direct  Blue  B extra  cone. 

or  Immedial  New  Blue  G cone. 
Sodium  sulphide  crystals 
Soda  ash 

Common  salt  or  desiccated 

Glauber’s  salt 


Starting  bath: 

5 —173/4  lbs 
15  -35*/2  lbs 
VJi—  2 lbs 

2 — 8 lbs 


Additions  for 
subsequent  lots : 

472-  15  lbs 
9 -30  lbs 

3/8—  1 lb 

3/8—  2 lbs 


Dyed  in  6 to  8 passages  at  boiling  temperature.  During  the  last 
passage  the  goods  are  squeezed  off  well  and  washed  straightaway  in  the 
rinsing  jigger. 

For  developing  the  Blue,  Immedial  New  Blue  G cone.,  when  the 
washing  is  completed,  is  aftertreated  for  20  minutes  at  about  80°  C. 
(175°  F.)  with  6 lbs  bluestone 

2 lbs  bichrome 
3 — 4 quarts  acetic  acid, 
and  then  rinsed  once  more. 


Light  Mode  Shades 

are  dyed  in  the  same  manner,  but  it  is  advisable  to  increase  the  amount 
of  sodium  sulphide  to  some  extent,  and  to  reduce  or  omit  the  Glauber’s 
salt.  In  the  case  of  material  difficult  to  penetrate,  it  is  well  to  add  to 
the  dyebath  1/2—  1 % Turkey-red  oil  or  Universal  oil  reckoned  on  the 
weight  of  the  goods. 


3 


Khaki,  for  instance,  is  dyed  in  the  following  manner: 

6 pieces  of  ticking,  weighing  107  lbs,  40  gallons  liquor. 

After  removing  the  size,  the  goods  are  boiled  in  two  passages  with 

10  oz  soda  ash  and 
2 lbs  sodium  sulphide  crystals; 

hereafter  they  are  dyed  hot 

for  light  Khaki  for  dark  Khaki 

with  137s  oz  Immedial  Yellow  Olive  G 1 lb  10  oz  Immedial  Yellow  Olive  G 
63/4  oz  Immedial  Cutch  0 7 oz  ImmedialYellow  Brown  EN 

1 lb  672  oz  sodium  sulphide  crystals  14  oz  Immedial  Brown  RR 

3 lbs  sodium  sulphide  crystals 

in  10  to  12  passages,  and  after  squeezing  are  rinsed  immediately  with  a 
copious  supply  of  water. 

The  aftertreatement  is  carried  out  with 

I72  lbs  bluestone 
172  lbs  bichrome 
172  quart  acetic  acid 

in  3 to  4 passages  in  a hot  bath;  finally,  the  goods  are  rinsed  once  more. 


DYEING  IN  THE  PADDING  MACHINE. 

The  dyeing  in  the  padding  machine  may  be  carried  out  by  two 
methods: 

1.  According  to  the  Jigger  Dyeing  Method 

The  goods  prepared  for  dyeing,  similarly  as  in  jigger  dyeing,  are 
passed  once  or  several  times  through  a trough  provided  with  several 
guiding  rollers,  then  squeezed  off,  and  cuttled,  or  rinsed  straightaway; 
see  Fig.  4. 


4 


2.  According  to  the  Padding  Method. 

This  method  has  been  found  very  serviceable,  especially  for  large 
production.  For  this  purpose  also,  a padding  machine  similar  to  Fig.  4 is 
used  except  that  it  is  provided  with  only  a very  small  trough.  In  a vessel 
placed  on  a higher  level  than  the  padding  machine  the  liquor  is  prepared 
according  to  the  shade  required,  and  heated  by  indirect  steam.  During 
the  dyeing  this  liquor  flows  continuously  into  the  little  trough,  to  best 
advantage  so  as  to  become  evenly  distributed  in  the  liquor;  see  Fig.  5. 


per  10  gallons  liquor 


The  dyebath  is  charged  as  follows: 

3U  oz  — 1 lb  dyestuff  for  light  shades 

1 — 3 lbs  dyestuff  for  medium  shades 
3—  6 lbs  dyestuff  for  dark  shades 
8 — 10  lbs  Immedial  Black  cone,  for  Black, 
as  well  as  with  double  the  amount  of  sodium  sulphide  crystals  as  of 
dyestuff  and  3 oz  Turkey-red  oil  per  10  gallons  liquor. 

As  a rule,  one  passage  is  sufficient  for  dyeing  the  goods,  two  or 
more  passages  being  required  in  the  case  of  deeper  shades  only. 

The  following  are  a few  examples: 


Dyeing  a Medium  Blue  with  Immedial  Indone 

according  to  Method  I. 

The  roller-box,  holding  about  40  gallons,  is  charged  for  about  100  lbs 
of  goods  with  8 lbs  Immedial  Indone  JBN  cone.  1 

16  lbs  sodium  sulphide  crystals  perm  gallons 
3'/2  quarts  Turkey-red  oil.  | 

The  goods,  after  being  freed  from  size  and  again  dried,  are  passed 
through  this  hot  dye  solution,  squeezed  off,  passed  through  the  air  over 
several  guiding  rollers  until  the  Blue  has  developed,  and  cuttled,  or  rinsed. 

According  to  the  depth  of  shade  required,  the  passage  is  repeated, 
either  once  or  several  times. 

The  bath  may  be  freshened  up  by  adding  more  concentrated  dye 
solutions. 


5 


I ' ' ■ -v  .WVWWVWVVWW TTTT^ 


Dyeing  of  Mode  Shades  in  the  Padding  Machine 

according  to  Method  II. 

The  stock  solution  is  charged  for  instance  with 

1 lb  Immedial  Dark  Brown  D cone.  1 

2 lbs  sodium  sulphide  crystals  l per  10  gallons  liquor. 

3 oz  Turkey-red  oil 

The  goods,  which  have  been  well  freed  from  size  and  dried  again, 
are  passed  through  the  hot  dye  solution  which  is  evenly  fed  into  the 
little  trough;  they  are  then  squeezed  off,  and  rinsed. 


DYEING  IN  THE  CONTINUOUS  MACHINE. 


In  the  continuous  machine  mostly  staple  shades  such  as  black, 
blue,  etc.  are  dyed.  The  construction  of  a continuous  dyeing  machine 
to  be  recommended  for  the  production  of  all  kinds  of  shades  is  shown 
in  Fig.  6. 


al 


a2 


a3 


No.  6 


(al)  and  (a 2)  are  two  large  roller-boxes,  each  holding  about  6G0  gallons 
of  dye-liquor.  The  partition  wall  between  the  two  vats  is  perforated  in  order  to 
keep  the  liquor  in  both  at  the  same  level;  (a3)  is  a rinsing  vat. 

Each  box  is  provided  with  an  efficient  pair  of  nippers,  both  of  which  are 
made  of  iron,  and  either  both  wrapped  with  cloth,  or  the  upper  one  coated  with 
rubber  and  the  lower  one  covered  with  cloth. 

Between  (a2)  and  (a3)  a system  of  guiding  rollers  is  arranged,  by  means 
of  which  the^goods  coming  pressed  off  from  the  dyebath  may  be  subjected  to  a 
short  or  slightly  prolonged  oxidation  in  the  air. 

Openers  are  fixed  where  the  goods  enter  the  bath  and  in  front  of  each 
pair  of  nippers  in  order  to  prevent  the  forming  of  folds. 

The  speed  is  so  regulated  as  to  allow  about  16  to  22  yards  to  pass  through 
the  machine  in  a minute,  about  11000  to  13000  yards  thus  being  dyed  in  a working 
day  of  10  hours’. 


6 


Fig.  7 shows  a similar  continuous  dyeing  machine. 


/ II  III  IV 

Fig.  7. 


The  first  two  vats  contain  the  dye  liquor,  the  third  and  fourth  serving  for 
the  rinsing.  Before  the  rinsing,  the  goods  may  be  taken  for  oxidation  over  the 
guiding  rollers  placed  above  the  dyeing  and  rinsing  vats. 


per  10  gallons  liquor. 


reckoned  on  the  weight 
of  the  goods  to  be  dyed. 


Immedial  Black 

on  Mercerised  Satteen  prepared  for  dyeing. 

Starting  Bath: 

2 — 272  lbs  Immedial  Black  NNG  cone. 

2 — 272  lbs  sodium  sulphide  crystals 
5 —8  oz  soda  ash 

I72 — 3 oz  Turkey-red  oil 

2 —272  lbs  common  salt  or  desiccated 

Glauber’s  salt 

During  the  dyeing,  the  dyebath  is  replenished  with 

5.5 —  6,5  0/o  Immedial  Black  NNG  cone. 

5.5 —  6,5o/0  sodium  sulphide  crystals 
0,5  0/0  soda  ash 
0,5o/o  Turkey-red  oil 

1 — 2 0/0  common  salt  or  desiccated 
Glauber’s  salt 

Dye  at  boiling  temperature  in  one  passage  only.  The  dyed  goods, 
after  pressing  off  well,  pass  along  to  the  rinsing  vats,  and  the  washing  is 
completed  quickly  in  a full  width-washing-machine,  being  finally  treated 
with  5—8  oz  acetate  or  formate  of  soda  per  10  gallons  liquor. 

„ , Immedial  Indone. 

Starting  B ath : 

6 oz  — D/2  lbs  Immedial  Indone  R cone. 

12  oz  — 3 lbs  sodium  sulphide  crystals 

3 — 6 oz  soda  ash 

172—  3 oz  Turkey-red  oil 

3—12  oz  glucose 

72—  2 lbs  common  salt  or  desiccated 

Glauber’s  salt 


per  10  gallons  liquor. 


7 


During  the  dyeing,  the  bath  is  replenished  with 
1,5-  8 o/o  Immedial  Indone  R cone. 

3 —16  o/o  sodium  sulphide  crystals 
0,5-  1 o/0  soda  ash 

0,5  o/o  Turkey-red  oil 

1 — 2 o/o  glucose 

2 - 3 o/o  common  salt  or  desiccated 

Glauber’s  salt 


calculated  on  the 
weight  of  Ihe  goods 
to  be  dyed. 


Dye  with  one  passage  at  50—60°  C.  (120 — 140°  F.).  After  passing 
the  two  dye  vats,  the  goods  are  run  over  a few  guiding  rollers  in  order 
to  oxidise,  and  then  into  the  rinsing  vats. 


AFTERTREATMENTS. 

Aftertreatment  with  Metallic  Salts. 

Immedial  Colours  as  a rule  do  not  require  any  aftertreatment  for 
enhancing  their  properties  of  fastness,  but  some  blue  and  mode  shades 
may  be  still  further  improved  in  fastness  to  light  and  washing  by  an 
aftertreatment  with 

2— 3  o/0  bluestone 
1/2 — 1 o/0  bichrome 

3— 4°/o  acetic  acid 

in  a bath  heated  to  70—80°  C.  (160—175°  F.).  The  bath  for  the  after- 
treatment  must  always  be  completely  clear. 

Aftertreatment  with  Acetate  and  Formate  of  Soda. 

This  treatment  is  principally  resorted  to  for  dyeings  produced  with 
Immedial  Black;  5—8  oz  acetate  of  soda  or  3—4 1/2  oz  formate  of  soda 
are  used  for  10  gallons  liquor,  being  added  to  the  last  rinsing  bath.  If 
the  goods  are  to  be  finished,  these  ingredients  may  also  be  added  to  the 
finishing  paste. 

Aftertreatment  with  Immedial  Developer. 

This  is  resorted  to  frequently  for  blue  Immedial  Colours  in  order 
to  enhance  their  brightness.  The  goods  are  dyed  as  usual  and  soaped. 
The  last  rinsing  bath  is  heated  to  40-50°  C.  (105—120°  F.)  and  1 — 1 '/2% 
Immedial  Developer,  previously  dissolved  in  warm  water,  are  then  added. 
The  goods  are  entered  cold,  the  bath  being  then  heated  gradually  to 
boiling  temperature;  finally  the  goods  are  rinsed. 

The  aftertreatment  with  the  Immedial  Developer  may  furthermore 
be  applied  to  very  good  advantage  for  developing  Immedial  Blue  and 
Immedial  New  Blue  in  cases  where  these  are  not  developed  by  smothering 
or  steaming.  The  developing  by  smothering  or  steaming  is  however  the 
most  advantageous  method  and  has  been  described  in  our  book  on  “Cotton 
Dyeing”,  pages  129-131. 

Shading  of  the  Immedial  Colours  with  Diamine  Colours  or  Basic  Colours. 

Certain  Diamine  or  Basic  Colours  may  be  used  for  shading  in  the 
Immedial  Colour  bath,  for  instance,  Diamine  Fast  Yellow  B,  Diamine 
Orange  B in  any  quantities;  Diamine  Red  4B,  Diamine  Brilliant  Scarlet  S, 
Diamine  Violet  Red,  Oxy  Diamine  Orange  G,  R,  Safranine,  all  brands, 
and  Tannin  Heliotrope  may  likewise  be  used,  but  in  very  small  quantities 
and  for  brightening  purposes  only. 

The  products  enumerated  have  the  property  to  exhaust  and  level 
well  in  a sodium  sulphide  bath. 


8 


Topping  with  Basic  Colours. 

For  enhancing  their  brightness,  the  Immedial  Colours  may  be  topped 
in  a fresh  bath  with  Basic  Colours,  the  following  brands  being  especially 
well  suited  for  this  purpose: 

for  Blue:  New  Methylene  Blue,  all  brands, 

Indazine  M,  Naphtindone  BB; 

for  Green:  Brilliant  Green  crystals  extra,  Solid  Green 

crystals  0 ; 

for  Brown:  Bismarck  Brown,  Chrysoidine,  Safranine,  all 

brands ; 

for  Claret  and  Violet:  Safranine,  Tannin  Heliotrope,  Methyl  Violet, 

all  brands; 

for  Yellow  and  Orange:  Thioflavine  T,  TCN,  Tannin  Orange  R. 

The  topping  is  carried  out  in  a cold  bath  charged  with  acetic  acid 
or  alum,  by  adding  the  dyestuff  in  several  portions,  heating  the  bath 
finally,  and  then  rinsing  in  cold  water. 


Without  guarantee. 


9 


The  percentages  stated  for  the  following  patterns  are  those  actually 
absorbed  by  the  fibre ; the  starting  bath  must  therefore,  accroding  to 
the  depth  of  the  shade,  be  charged  with  correspondingly  larger  quantities. 
Exact  indications  will  be  found  in  our  “Manual  of  Dyeing”,  Vol.  I, 
pages  16-22. 


IMMEDIAL  COLOURS  (Self  Shades). 


1. 

2 % Immedial  Yellow  GG  pat. 

2. 

4 % Immedial  Yellow  GG  pat. 

3. 

4 % Immedial  Yellow  D pat. 

4. 

8 % Immedial  Yellow  D pat. 

' 5. 

3 % Immedial  Orange  C pat. 

6. 

6 % Immedial  Orange  C pat. 

7. 

2.5%  Immedial  Cutch  O pat. 

8. 

6 % Immedial  Cutch  0 pat. 

9. 

2.5%  Immedial  Cutch  R pat. 

10. 

8 % Immedial  Cutch  R pat. 

11. 

2,5%  Immedial  Cutch  BGG  pat. 

12. 

6 % Immedial  Cutch  BGG  pat. 

13. 

2,5%  Immedial  Cutch  BG  pat. 

14. 

8 % Immedial  Cutch  BG  pat. 

15. 

2,5%  Immedial  Cutch  G pat. 

16. 

6 % Immedial  Cutch  G pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


1MMEDIAL  COLOURS  (Self  Shades). 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


i 


IMMEDIAL  COLOURS  (Self  Shades). 


17. 

2,5%  Immedial  Yellow  Brown  EN  pat. 

18. 

6 % Immedial  Yellow  Brown  EN  pat. 

19. 

2,5%  Immedial  Brown  BR. 

20. 

6 % Immedial  Brown  BR. 

• 21. 

2,5%  Immedial  Brown  RR  pat. 

22. 

6 % Immedial  Brown  RR  pat. 

22. 

2,5%  Immedial  Dark  Brown  A pat. 

24. 

6 % Immedial  Dark  Brown  A pat. 

25. 

2,5%  Immedial  Dark  Brown  D cone.  pat. 

26. 

6 % Immedial  Dark  Brown  D cone,  pat 

27. 

2,5%  Immedial  Brown  W cone.  pat. 

28. 

6 % Immedial  Brown  W cone.  pat. 

29. 

2,5%  Immedial  Prune  S pat. 

30. 

6 % Immedial  Prune  S pat. 

31. 

4 % Immedial  Red  Brown  3R  pat. 

32. 

8 % Immedial  Red  Brown  3R  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


CASSELLA  COLOK  COMPANY,  NEW  YOKE. 


IMMEDIAL  COLOURS  (Self  Shades). 


33. 

2,5%  Immedial  Maroon  B cone.  pat. 

34. 

G % Immedial  Maroon  B cone.  pat. 

35. 

2,5%  Immedial  Bordeaux  GF  cone.  pat. 

36. 

8 % Immedial  Bordeaux  GF  cone.  pat. 

37. 

4 % Immedial  Violet  CB  pat. 

38. 

8 % Immedial  Violet  CB  pat. 

39. 

4 % Immedial  Violet  CR  pat. 

40. 

8 % Immedial  Violet  CR  pat. 

41. 

4 % Immedial  Purple  C pat. 

42. 

8 % Immedial  Purple  C pat. 

43. 

4 % Immedial  Violet  C pat. 

44. 

8 % Immedial  Violet  C pat. 

45. 

2,5%  Immedial  Khaki  G pat. 

46. 

4 % Immedial  Khaki  G pat. 

47. 

1,5%  Immedial  Khaki  D pat. 

48. 

3 % Immedial  Khaki  D pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IMMEDIAL  COLOURS  (Self  Shades). 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


hi 


IMMEDIAL  COLOURS  (Self  Shades). 


49. 

3%  Immedial  Yellow  Olive  5G  pat. 

50. 

8%  Immedial  Yellow  Olive  5G  pat. 

51. 

3%  Immedial  Yellow  Olive  G pat. 

52. 

8n/o  Immedial  Yellow  Olive  G pat. 

’ 53. 

3%  Immedial  Olive  3G. 

54. 

8%  Immedial  Olive  3G. 

55. 

3%  Immedial  Olive  GG  pat. 

56. 

8%  Immedial  Olive  GG  pat. 

57. 

3%  Immedial  Olive  B pat. 

58. 

8%  Immedial  Olive  B pat. 

59. 

2%  Immedial  Brilliant  Green  G extra  pat. 

60. 

6%  Immedial  Brilliant  Green  G extra  pat. 
61. 

2%  Immedial  Green  GG  extra  pat. 

62. 

6%  Immedial  Green  GG  extra  pat. 

63. 

3%  Immedial  Green  GGX  cone.  pat. 

64. 

8%  Immedial  Green  GGX  cone.  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IV 


IMMEDIAL  COLOURS  (Self  Shades). 


65. 

3%  Immedial  Green  BB  extra  pat. 

66. 

8%  Immedial  Green  BB  extra  pat. 

67. 

3%  Immedial  Green  BBX  cone.  pat. 

68. 

8%  Immedial  Green  BBX  cone.  pat. 

69. 

3%  Immedial  Green  Blue  CV  pat. 

70. 

8%  Immedial  Green  Blue  CV  pat. 

71. 

3%  Immedial  Deep  Green  G pat. 

72. 

8%  Immedial  Deep  Green  G pat. 

73. 

3 % Immedial  Dark  Green  B. 

74. 

8 % Immedial  Dark  Green  B. 

75. 

2,5%  Immedial  Sky  Blue  Powder  cone.  pat. 
aftertreated  with: 
bluestone  and  blchrome. 

76. 

12  % Immedial  Sky  Blue  Powder  cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

77. 

2,5%  Immedial  Indone  3B  cone.  pat. 

78. 

6 % Immedial  Indone  3B  cone.  pat. 

79. 

2 % Immedial  Indone  BBF  cone.  pat. 

80. 

6 % Immedial  Indone  BBF  cone.  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IMMEDIAL  COLOURS  (Self  Shades). 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


v 


IMMEDIAL  COLOURS  (Self  Shades). 


81. 

2,5%  Immedial  Indone  BP  cone.  pat. 

82. 

6 % Immedial  Indone  BP  cone.  pat. 

83. 

2,5%  Immedial  Indone  BN  cone.  pat. 

84. 

6 % Immedial  Indone  BN  cone.  pat. 

85. 

2,5%  Immedial  Indone  JBN  cone.  pat. 

86. 

6 % Immedial  Indone  JBN  cone.  pat. 

87. 

2,5%  Immedial  Indone  JBF  cone.  pat. 

88. 

6 % Immedial  Indone  JBF  cone.  pat. 

89. 

2,5%  Immedial  Indone  R cone.  pat. 

90. 

7 % Immedial  Indone  R cone.  pat. 

91. 

2,5%  Immedial  Indone  RR  cone.  pat. 

92. 

7 % Immedial  Indone  RR  cone.  pat. 

93. 

2,5%  Immedial  Indone  Violet  B cone.  pat. 

94. 

7 % Immedial  Indone  Violet  B cone.  pat. 

95. 

2,5%  Immedial  Indone  RB  cone.  pat. 

96. 

7 % Immedial  Indone  RB  cone.  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IMMEDIAL  COLOURS  (Self  Shades). 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


VI 


IMMEDIAL  COLOURS  (Self  Shades). 


97. 

2,5%  Immedial  Indone  RG  cone.  pat. 

98. 

8 % Immedial  Indone  RG  cone.  pat. 

99. 

3 % Immedial  Indogene  GCL  cone.  pat. 

100. 

7 % Immedial  Indogene  GCL  cone.  pat. 

101. 

3 % Immedial  Indogene  BCL  cone.  pat. 

102. 

7 % Immedial  Indogene  BCL  cone.  pat. 

103. 

3 % Immedial  Indogene  RCL  cone.  pat. 

104. 

7 % Immedial  Indogene  RCL  cone.  pat. 

105. 

3%  Immedial  Indogene  RRCL  cone.  pat. 

106. 

7%  Immedial  Indogene  RRCL  cone.  pat. 

107. 

3%  Immedial  Indogene  B cone.  pat. 

108. 

7%  Immedial  Indogene  B cone.  pat. 

109. 

3%  Immedial  Direct  Blue  OD  pat. 

110. 

8%  Immedial  Direct  Blue  OD  pat. 

111. 

3%  Immedial  Direct  Blue  B pat. 

112. 

8%  Immedial  Direct  Blue  B pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IMMEDIAL  COLOURS  (Self  Shades). 

97 

105 

98 

106 

99 

107 

100 

Bi 

108 

101 

109 

102 

! 

110 

103 

■Hi 

111 

104 

112 

CASSELLA  COLOR  COMPANY,  NEW  YORK. 

VII 


IMMEDIAL  COLOURS  (Self  Shades). 


113. 

3 % Immedial  Direct  Blue  JB  pat. 

114. 

8 % Immedial  Direct  Blue  JB  pat. 

115. 

3 % Immedial  Direct  Blue  R pat. 

116. 

8 % Immedial  Direct  Blue  R pat. 


. 117. 

2 % Immedial  Direct  Blue  4B 

extra  cone.  pat. 


118. 

5,5%  Immedial  Direct  Blue  4B 

extra  cone.  pat. 


119. 

2 % Immedial  Direct  Blue  BB 

extra  cone.  pat. 

120. 

5,5%  Immedial  Direct  Blue  BB 

extra  cone.  pat. 

121. 

2 % Immedial  Direct  Blue  FCL 

extra  cone.  pat. 


122. 

5 % Immedial  Direct  Blue  FCL 

extra  cone.  pat. 


123. 

2,5%  Immedial  Direct  Blue  JND 

extra  cone.  pat. 

124. 

7 % Immedial  Direct  Blue  JND 

extra  cone.  pat. 

125. 

2,5%  Immedial  New  Blue  G cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 


126. 

7 % Immedial  New  Blue  G cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 


127. 

0,5%  Immedial  Black  NNG  cone.  pat. 

128. 

6,5%  Immedial  Black  NNG  cone.  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IM MEDIAL  COLOURS  (Self  Shades). 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


VIII 


IMMEDIAL  COLOURS  (Self  Shades). 


129. 

0,5  % Immedial  Black  NBB  cone.  pat. 


130. 

6,5  % Immedial  Black  NBB  cone.  pat. 


131. 

0,5  % Immedial  Brilliant  Black  6BG 

cone.  pat. 

132. 

6,5  % Immedial  Brilliant  Black  6BG 

cone,  pat, 

• 133. 

0,35%  Immedial  Carbon  B pat. 


134. 

4,5  % Immedial  Carbon  B pat. 


135. 

0,35%  Immedial  Brilliant  Carbon  FG  pat. 


136. 

5 % Immedial  Brilliant  Carbon  FG  pat. 


137. 

0,5  % Immedial  Brilliant  Black  5BV 

cone.  pat. 

138. 

6,5  % Immedial  Brilliant  Black  5BV 

cone.  pat. 

139. 

0,5  % Immedial  Brilliant  Black  8BG 

cone.  pat. 

140. 

6,5  % Immedial  Brilliant  Black  8BG 

cone.  pat. 

141. 

0,5  % Immedial  Black  NLN  cone. 


142. 

6,5  % Immedial  Black  NLN  cone. 


143. 

0,35%  Immedial  Carbon  R. 


144. 

4,5  % Immedial  Carbon  R. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


IX 


INDIGO  AND  MODE  SHADES  PRODUCED  WITH  IMMEDIAL 

COLOURS. 

3 % 

Immedial 

145. 

Indone  JBN  cone.  pat. 

0,2  % 

Immedial 

Green  BB  extra  pat. 

4 % 

Immedial 

146. 

Indone  JBN  cone.  pat. 

0,4  % 

Immedial 

Green  BB  extra  pat. 

4 % 

Immedial 

147. 

Indone  JBN  cone.  pat. 

0,7  % 

Immedial 

Direct  Blue  B extra  cone. 

0,2  % 

Immedial 

Green  BB  extra  pat.  fpat. 

4,5  % 

Immedial 

148. 

Indone  JBN  cone.  pat. 

1 % 

Immedial 

Direct  Blue  B extra  cone. 

3.  % 

Immedial 

pat. 

149. 

Indone  JBN  cone.  pat. 

2,6  % 

Immedial 

Indone  R cone.  pat. 

0,7  % 

Immedial 

Direct  Blue  B extra  cone. 

4 % 

Immedial 

pat. 

150. 

Indone  JBN  cone.  pat. 

3 % 

Immedial 

Indone  R cone.  pat. 

1,5  % 

Immedial 

Direct  Blue  B extra  cone. 

3,75% 

Immedial 

pat. 

151. 

Indone  JBN  cone.  pat. 

3,5  % 

Immedial 

Indone  R cone.  pat. 

2,4  % 

Immedial 

Direct  Blue  B extra  cone. 

5 % 

Immedial 

pat. 

152. 

Indone  JBN  cone.  pat. 

4,5  % 

Immedial 

Indone  R cone.  pat. 

3,5  % 

Immedial 

Direct  Blue  B extra  cone. 

0,5  % 

Immedial 

pat. 

153. 

Indogene  GCL  cone.  pat. 

0,04% 

Immedial 

Green  BB  extra  pat. 

1,2  % 

Immedial 

154. 

Indogene  GCL  cone.  pat. 

0,12% 

Immedial 

Green  BB  extra  pat. 

3 % 

Immedial 

155. 

Indogene  GCL  cone.  pat. 

0,08% 

Immedial 

Green  BB  extra  pat. 

2,25% 

Immedial 

156. 

Indogene  GCL  cone.  pat. 

0,25% 

Immedial 

Green  BB  extra  pat. 

4 % 

Immedial 

157. 

Indogene  GCL  cone.  pat. 

1,2  % 

Immedial 

Green  BB  extra  pat. 

2 % 

Immedial 

158. 

Green  Blue  CV  pat. 

0,08% 

Immedial 

Yellow  Olive  5G  pat. 

4,75% 

Immedial 

159. 

Green  Blue  CV  pat. 

0,35% 

Immedial 

Cutch  O pat. 

5,5  % 

Immedial 

160. 

Green  Blue  CV  pat. 

0,7  % 

Immedial 

Cutch  O pat. 

CASSELLA  COLOR  COMPANY,  NEW  YOKK. 


INDIGO  AND  MODE  SHADES  PRODUCED  WITH  IMMEDIAL  COLOURS. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


_ 


x 


MODE  SHADES  PRODUCED  WITH  IMMEDIAL  COLOURS.. 


161. 

0,16%  Immedial  Carbon  B pat. 

0,1  % Immedial  Direct  Blue  B pat. 


162. 

0,16%  Immedial  Carbon  B pat. 

0,2  % Immedial  Dark  Brown  D cone.  pat. 


163. 

0,2  % Immedial  Carbon  B pat. 
0,35%  Immedial  Brown  BR. 


164. 

0,45%  Immedial  Carbon  B pat. 
0,24%  Immedial  Brown  BR. 


165. 

0,25%  Immedial  Carbon  B pat. 

0,4  % Immedial  Dark  Brown  D cone.  pat. 


166. 

1,2  % Immedial  Dark  Green  B 
1,2  % Immedial  Direct  Blue  B pat. 


167. 

1 % Immedial  Direct  Blue  B pat. 

0,45%  Immedial  Black  NBB  cone.  pat. 


168. 

3,5  % Immedial  Direct  Blue  B pat. 

0,7  % Immedial  Black  NBB  cone.  pat. 


169. 

0,07%  Immedial  Carbon  B pat. 

0,05%  Immedial  Bordeaux  GP  cone.  pat. 


170. 

0,08%  Immedial  Carbon  B pat. 

0,08%  Immedial  Bordeaux  GP  cone.  pat. 


171. 

0,7  % Immedial  Carbon  B pat. 
0,7  % Immedial  Prune  S pat. 


172. 

0,25%  Immedial  Carbon  B pat. 

0,08%  Immedial  Dark  Brown  D cone.  pat. 


173. 

0,2  % Immedial  Carbon  B pat. 

0,22%  Immedial  Dark  Brown  D cone.  pat. 
0,3  % Immedial  Cutcb  G pat. 


174. 

0,6  % Immedial  Dark  Brown  D cone.  pat. 
0,35%  Immedial  Olive  B pat. 


175. 

0,7  % Immedial  Cutch  G pat. 

0,2  % Immedial  Carbon  B pat. 

0,5  % Immedial  Dark  Brown  D cone.  pat. 


176. 

1,35%  Immedial  Cutch  G pat. 

0,22%  Immedial  Carbon  B pat. 

0,22%  Immedial  Dark  Brown  D cone.  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


XI 


MODE  SHADES  PRODUCED  WITH  IMMEDIAL  COLOURS. 


177. 

0,35%  Immedial  Indogene  GCL  cone.  pat. 
1 % Immedial  Green  GG  extra  pat. 


178. 

0,65%  Immedial  Direct  Blue  B pat. 
0,7  % Immedial  Green  BB  extra  pat. 


179. 

2 % Immedial  Direct  Blue  B pat. 

2,4  % Immedial  Indogene  GCL  cone.  pat. 


180. 

0,5  % Immedial  Indogene  GCL  cone.  pat. 


181. 

1,3  % Immedial  Indone  R cone.  pat. 
0,5  % Immedial  Direct  Blue  B pat. 


182. 

3 % Immedial  Indogene  GCL  cone.  pat. 

0,6  % Immedial  Green  BB  extra  pat. 


183. 

6,6  % Immedial  Indogene  GCL  cone.  pat. 
0,7  % Immedial  Green  BB  extra  pat. 


184. 

2 % Immedial  Direct  Blue  B pat. 

0,5  % Immedial  Black  NBB  cone.  pat. 


185. 

0,4  % Immedial  Green  GG  extra  pat. 
0,08%  Immedial  Direct  Blue  B pat. 


186. 

2 % Immedial  Indogene  GCL  cone.  pat. 

1,5  % Immedial  Green  BB  extra  pat. 


187. 

3 % Immedial  Indogene  GCL  cone.  pat. 

2,75%  Immedial  Green  BB  extra  pat. 


188. 

4 % Immedial  Olive  GG  pat. 

0,7  % Immedial  Green  GG  extra  pat. 
1,2  % Immedial  Yellow  D pat. 


189. 

3 % Immedial  Green  GG  extra  pat. 

2,4  % Immedial  Yellow  D pat. 


190. 

4,6  % Immedial  Olive  GG  pat. 

1.4  % Immedial  Green  GG  extra  pat. 

1.5  % Immedial  Yellow  D pat. 


191. 

1.5  % Immedial  Green  GG  extra  pat. 

6.6  % Immedial  Yellow  Olive  5G  pat. 
2,4  % Immedial  Dark  Green  B. 


192. 

7 % Immedial  Deep  Green  G pat. 

0,35%  Immedial  Cutch  O pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


XII 


MODE  SHADES  PRODUCED  WITH  IMMEDIAL  COLOURS. 


193. 

0,6  % Immedial  Bordeaux  GP  cone.  pat. 
0,3  % Immedial  Orange  C pat. 


194. 

0,08%  Immedial  Bordeaux  GP  cone.  pat. 
0,45%  Immedial  Orange  C pat. 

195. 

1 % Immedial  Cutch  O pat. 

196. 

2,4  % Immedial  Cutch  O pat. 

1,2  % Immedial  Olive  B pat. 


197. 

4 • % Immedial  Cutch  O pat. 
0,2  % Immedial  Dark  Green  B. 


198. 

2,4  % Immedial  Orange  C pat. 

0,5  % Immedial  Bordeaux  GF  cone.  pat. 


199. 

3 % Immedial  Yellow  Brown  EN  pat. 

1,5  % Immedial  Bordeaux  GF  cone,  pat 


200. 

3,75%  Immedial  Orange  C pat. 

2,25%  Immedial  Bordeaux  GF  cone.  pat. 
0,4  % Immedial  Catechu  O pat. 


201. 

5,5%  Immedial  Orange  C pat. 

1,5%  Immedial  Bordeaux  GF  cone.  pat. 

202. 

2  % Immedial  Orange  C pat. 

4 % Immedial  Bordeaux  GF  cone.  pat. 

203. 

6 % Immedial  Bordeaux  GF  cone.  pat. 
1,5%  Immedial  Orange  C pat. 


204. 

3  % Immedial  Yellow  Olive  5G  pat. 
1,5%  Immedial  Cutch  O pat. 


205. 

4  % Immedial  Orange  C pat. 

2 % Immedial  Green  GG  extra  pat. 


206. 

7 % Immedial  Yellow  Olive  5G  pat. 
2,4%  Immedial  Green  GG  extra  pat. 


207. 

6 % Immedial  Yellow  Olive  5G  pat. 
4 % Immedial  Green  GG  extra  pat. 


208. 

6 % Immedial  Green  Blue  CV  pat. 
4 % Immedial  Yellow  Olive  5G  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


XIII 


MODE  SHADES  PRODUCED  WITH  IMMEDIAL  COLOURS. 


209. 

1,2  % Immedial  Direct  Blue  B pat. 

0,5  % Immedial  Green  BB  extra  pat. 


210. 

0,8  % Immedial  Direct  Blue  B pat. 
0,24%  Immedial  Carbon  B pat. 


211. 

0,7  % Immedial  Carbon  B pat. 

0,7  % Immedial  Direct  Blue  B pat. 


212. 

3 % Immedial  Dark  Green  B 

1,5  % Immedial  Black  NNG  cone.  pat. 


. 213. 

2,4  % Immedial  Black  NNG  cone.  pat. 
0,0  % Immedial  Dark  Green  B. 


214. 

6,0  % Immedial  Yellow  Brown  EN  pat. 

1,5  % Immedial  Dark  Green  B. 


215. 

5 % Immedial  Dark  Brown  D cone.  pat. 

2 % Immedial  Cutch  O pat. 


216. 

3,5  % Immedial  Dark  Brown  D cone.  pat. 

1,2  % Immedial  Black  NNG  cone.  pat. 

217. 

0,8  % Immedial  Violet  CR  pat. 

218. 

2 % Immedial  Violet  CR  pat. 

219. 

2 % Immedial  Violet  CR  pat 

0,7  % Immedial  Bordeaux  GF  cone.  pat. 


220. 

2,1  % Immedial  Violet  CR  pat. 

2,4  % Immedial  Bordeaux  GF  cone.  pat. 


221. 

0,35%  Immedial  Brown  RR  pat. 
0,35%  Immedial  Brown  BR. 


222. 

1,35%  Immedial  Brown  RR  pat. 
0,22%  Immedial  Brown  BR. 


223. 

3,35%  Immedial  Brown  RR  pat. 

1,2  % Immedial  Brown  BR. 


224. 

2,75%  Immedial  Prune  S pat. 

0,7  % Immedial  Bordeaux  GF  cone.  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


XIV 


MODE  SHADES  PRODUCED  WITH  IMMEDIAL  COLOURS. 


225. 

0,24%  Immedial  Cutcli  0 pat. 

0,16%  Immedial  Bordeaux  GP  cone.  pat. 


226. 

1,5  % Immedial  Cutch  O pat. 

0,2  % Immedial  Bordeaux  GF  cone.  pat. 


227. 

4 % Immedial  Cutcli  O pat. 

1,2  % Immedial  Yellow  Olive  5G  pat. 


228. 

0,5  % Immedial  Dark  Brown  D cone.  pat. 
0,3  % Immedial  Yellow  Brown  EN  pat. 


229. 

0,7  % Immedial  Dark  Brown  D cone.  pat. 
0,7  % Immedial  Yellow  Brown  EN  pat. 


230. 

0,7  % Immedial  Dark  Brown  D cone.  pat. 
0,5  % Immedial  Yellow  Brown  EN  pat. 


231. 

1,2  % Immedial  Dark  Brown  D cone.  pat. 
6,6  % Immedial  Cutch  G pat. 

0,9  % Immedial  Dark  Green  B. 


232. 

5.5  % Immedial  Cutch  O pat. 

1.5  % Immedial  Brown  W cone.  pat. 


233. 


0,5% 

Immedial 

Maroon  B cone.  pat. 

0,6% 

Immedial 

Cutch  BGG  pat. 

234. 

2,5% 

Immedial 

Purple  C pat. 

235. 

1,2% 

Immedial 

Prune  S pat. 

1,3% 

Immedial 

Bordeaux  GP  cone.  pat. 

236. 

2 % 

Immedial 

Violet  CR  pat. 

1 % 

Immedial 

Prune  S pat. 

237. 

4 % 

Immedial 

Prune  S pat. 

238. 

4 % 

Immedial 

Bordeaux  GP  cone.  pat. 

3 % 

Immedial 

Prune  S pat. 

239. 

5 % 

Immedial 

Bordeaux  GP  cone.  pat. 

4 % 

Immedial 

Prune  S pat. 

240. 

6 % 

Immedial 

Brown  BR  pat. 

2 % 

Immedial 

Black  NNG  cone.  pat. 

CASSELLA  COLOR  COMPANY,  NEW  YORK. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


MODE  SHADES  PRODUCED  WITH  IMMEDIAL 

COLOURS. 

241. 

3 % 

Immedial 

Yellow  GG  pat. 

1 % 

Immedial 

Brilliant  Green  G extra  pat. 

242. 

2,75% 

Immedial 

Yellow  GG  pat. 

0,6  % 

Immedial 

Brilliant  Green  G extra  pat. 

243. 

5,5  % 

Immedial 

Yellow  Olive  G pat. 

0,7  % 

Immedial 

Brilliant  Green  G extra  pat. 

244. 

5,5  % 

Immedial 

Yellow  Olive  5G  pat. 

0,32% 

Immedial 

Brilliant  Green  G extra  pat. 

245. 

4,35% 

Immedial 

Yellow  Olive  5G  pat. 

0,6  % 

Immedial 

Brilliant  Green  G extra  pat. 

246. 

5,5  % 

Immedial 

Yellow  Olive  5G  pat. 

2 % 

Immedial 

Brilliant  Green  G extra  pat. 

247. 

5,5  % 

Immedial 

Yellow  Olive  5G  pat. 

3 % 

Immedial 

Green  Blue  CV  pat. 

248. 

5,5  % 

Immedial 

Green  Blue  CV  pat. 

4 % 

Immedial 

Yellow  Olive  5G  pat. 

249. 

0,5  % 

Immedial 

Dark  Brown  D cone.  pat. 

0,58% 

Immedial 

Cutch  G pat. 

250. 

0,6  % 

Immedial 

Olive  B pat. 

0,35% 

Immedial 

Dark  Brown  D cone.  pat. 

251. 

1,2  % 

Immedial 

Dark  Brown  D cone.  pat. 

0,32% 

Immedial 

Yellow  Brown  EN  pat. 

252. 

2,4  % 

Immedial 

Cutch  G pat. 

0,65% 

Immedial 

Dark  Brown  D cone.  pat. 

253. 

1 % 

Immedial 

Olive  B pat. 

0,62% 

Immedial 

Cutch  G pat. 

254. 

1,5  % 

Immedial 

Cutch  G pat. 

1 % 

Immedial 

Olive  B pat. 

0,22% 

Immedial 

Dark  Brown  D cone.  pat. 

255. 

2,1  % 

Immedial 

Olive  B pat. 

0,65% 

Immedial 

Dark  Brown  D cone.  pat. 

0,32% 

Immedial 

Cutch  G pat. 

256. 

2,3  % 

Immedial 

Yellow  Brown  EN  pat. 

1,5  % 

Immedial 

Dark  Green  B 

0,35% 

Immedial 

Dark  Brown  D cone.  pat. 

CASSELLA  COLOR  COMPANY,  NEW  YORK. 

CASSELLA  COLOR  COMPANY,  NEW  YORK. 


UPHOLSTERY  CLOTH  DYED  WITH  IMMEDIAL  COLOURS,  AFTERTREATED. 


257. 

0,15  % Immedial  Dark  Brown  D cone.  pat. 
0,025%  Immedial  Yellow  Olive  5G  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

258. 

0,48  % Immedial  Green  GG  extra  pat. 

0,08  7o  Immedial  Yellow  Olive  5G  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

259. 

1,2  % Immedial  Orange  C pat. 

0,35  % Immedial  Dark  Brown  D cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

260. 

1,2  % Immedial  Indogene  GCL  cone.  pat. 

0,8  % Immedial  Indone  Violet  B cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

261. 

6,5  % Immedial  Bordeaux  GP  cone,  pat 
• aftertreated  with: 

bluestone  and  bichrome. 

262. 

0,35  % Immedial  Direct  Blue  B pat. 

0,25  % Immedial  Carbon  B pat. 
aftertreated  with: 
bluestone  and  bichrome. 

263. 

6.5  % Immedial  Yellow  Olive  5G  pat. 

3 % Immedial  Green  GG  extra  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

264. 

5.5  % Immedial  Green  GG  extra  pat. 

2.5  % Immedial  Yellow  Olive  5G  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

265. 

4 % Immedial  Yellow  Brown  EN  pat. 

2,4%  Immedial  Dark  Brown  D cone.  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

266. 

6,6%  Immedial  Cutch  O pat. 

2 % Immedial  Brown  BR 

aftertreated  with: 
bluestone  and  bichrome. 

267. 

7,5%  Immedial  Violet  CR  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

268. 

3 % Immedial  Yellow  Brown  EN  pat. 

1,2%  Immedial  Dark  Brown  D cone.  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

269. 

3 % Immedial  Bordeaux  GP  cone.  pat. 

1 % Immedial  Violet  CR  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

270. 

2 % Immedial  Khaki  G pat. 

aftertreated  with: 
bluestone  and  bichrome. 

271. 

3,5%  Immedial  Indogene  GCL  cone.  pat. 
1,5%  Immedial  Green  BB  extra  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

272. 

2 % Immedial  Violet  CR  pat. 

0,7%  Immedial  Carbon  B pat. 

aftertreated  with: 
bluestone  and  bichrome. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


u 


PHOLSTERY  CLOTH  DYED 


WITH  DIME  DIAL  COLOURS,  AFTER  TREATED. 


XVII 


CASSELLA  COLOR  COMPANY,  NEW  YORK 


KHAKI  AND  “FIELD  GREY”  DYED  WITH  IMMEDIAL  COLOURS. 


273. 

2 % Immedial  Khaki  G pat. 

0,15%  Immedial  Dark  Green  B 

aftertreated  with: 
bluestone  and  biehrome. 

274. 

1 % Immedial  Khaki  D pat. 

0,7  % Immedial  Khaki  G pat. 

0,08%  Immedial  Dark  Green  B 
aftertreated  with: 
bluestone  and  bichrome. 

275. 

2,  % Immedial  Khaki  G pat. 

1,25%  Immedial  Yellow  D pat. 

aftertreated  with: 
bluestone  and  bichrome. 

276. 

1.5  % Immedial  Khaki  D pat. 

aftertreated  with: 
bluestone  and  bichrome. 

277. 

3 % Immedial  Yellow  Olive  5G  pat. 

0,5  % Immedial  Dark  Green  B 

aftertreated  with: 

• bluestone  and  bichrome. 

278. 

2.5  % Immedial  Khaki  D pat. 

0,06%  Immedial  Dark  Green  B 

aftertreated  with: 
bluestone  and  bichrome. 

279. 

0,7  % Immedial  Yellow  Olive  5G  pat. 

0,7  % Immedial  Brown  BR 
0,12%  Immedial  Dark  Green  B 
aftertreated  with: 
bluestone  and  bichrome. 

280. 

0,8  % Immedial  Yellow  Olive  5G  pat. 

0,8  % Immedial  Brown  BR 
0,1  % Immedial  Dark  Green  B 
aftertreated  with: 
bluestone  and  bichrome. 

281. 

0,25%  Immedial  Green  BB  extra  pat. 

0,08%  Immedial  Carbon  B pat. 

aftertreated  with: 
bluestone  and  bichrome. 

282. 

0,25%  Immedial  Carbon  B pat 
0,2  % Immedial  Dark  Brown  D cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

283. 

0,6  % Immedial  Dark  Brown  D cone.  pat. 
0,3  % Immedial  Yellow  Brown  EN  pat. 
0,08%  Immedial  Carbon  B pat. 
aftertreated  with: 
bluestone  and  bichrome. 

284. 

1.5  % Immedial  Olive  B pat. 

0,6  % Immedial  Dark  Green  B pat. 

0,12%  Immedial  Black  NNG  cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

285. 

1 % Immedial  Dark  Brown  D cone.  pat. 

0,75%  Immedial  Dark  Green  B 
aftertreated  with: 
bluestone  and  bichrome. 

286. 

0,6  % Immedial  Direct  Blue  B pat. 

0,56%  Immedial  Dark  Green  B 
0,5  % Immedial  Green  BB  extra  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

287. 

0,7  % Immedial  Black  NLN  cone. 

0,16%  Immedial  Yellow  Olive  G pat. 
aftertreated  with: 
bluestone  and  bichrome. 

288. 

3.5  % Immedial  Dark  Brown  A pat. 

1.5  % Immedial  Cutch  G pat. 

aftertreated  with: 
bluestone  and  bichrome. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


XVIII 


TENT  CLOTH  AND  MOLESKIN  DYED  WITH  IMMEDIAL  COLOURS, 

AFTERTREATED. 


289. 

1,2  % Immedial  Green  GG  extra  pat. 

0,25%  Immedial  Yellow  Olive  5G  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

290. 

0,7  % Immedial  Green  Blue  CV  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

291. 

3.5  % Immedial  Bordeaux  GF  cone.  pat. 
0,8  % Immedial  Cutch  0 pat. 

aftertreated  with: 
bluestone  and  bichrome. 

292. 

4 % Immedial  Maroon  B cone.  pat. 

2 % Immedial  Cutch  O pat. 

aftertreated  with: 
bluestone  and  bichrome. 

293. 

6 % Immedial  Maroon  B cone.  pat. 

3 % Immedial  Cutch  O pat. 

aftertreated  with: 

' bluestone  and  bichrome. 

294. 

2 % Immedial  Dark  Green  B 

4 % Immedial  Yellow  Brown  EN  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

295. 

4 % Immedial  Green  Blue  CV  pat. 

2.4  % Immedial  Yellow  Olive  G pat. 

aftertreated  with: 
bluestone  and  bichrome. 

296. 

8 % Immedial  Brown  BR 

aftertreated  with: 
bluestone  and  bichrome. 

297. 

0,3  % Immedial  Yellow  Olive  G pat. 

0,2  % Immedial  Dark  Green  B 
aftertreated  with: 
bluestone  and  bichrome. 

298. 

1,2  % Immedial  Yellow  Brown  EN  pat. 

0,6  % Immedial  Dark  Brown  D cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

299. 

1,2  % Immedial  Dark  Green  B 
0,7  % Immedial  Dark  Brown  D cone.  pat. 
aftertreated  with: 
bluestone  and  bichrome. 

300. 

2 % Immedial  Dark  Brown  D cone.  pat. 
0,35%  Immedial  Carbon  B pat. 

aftertreated  with: 
bluestone  and  bichrome. 

301. 

6.6  % Immedial  Yellow  Olive  5G  pat. 

3 % Immedial  Dark  Green  B 

aftertreated  with: 
bluestone  and  bichrome. 

302. 

8 % Immedial  Yellow  Olive  5G  pat. 

1.5  % Immedial  Dark  Green  B 

aftertreated  with: 
bluestone  and  blchrome. 

303. 

4 % Immedial  Brown  BR 

3.5  % Immedial  Yellow  Brown  EN  pat. 

0,7  % Immedial  Carbon  B pat. 

aftertreated  with: 
bluestone  and  bichrome. 

304. 

4 % Immedial  Brown  BR 

3 % Immedial  Yellow  Brown  EN  pat. 

1.5  % Immedial  Carbon  B pat. 

aftertreated  with: 
bluestone  and  bichrome. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


TENT  CLOTH  AND  MOLESKIN  DYED  WITH  IMMEDIAL  COLOURS" 

AFTERTREATED. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


XIX 


WORKMEN’S  SUITINGS  DYED  WITH  IMMEDIAL  COLOURS, 
DIRECT  AND  AFTERTREATED. 

5,5% 

0,5% 

305. 

Immedial  Indone  JBN  cone.  pat. 
Immedial  Direct  Blue  B pat. 

6 % 
2 % 

306. 

Immedial  Indone  JBN  cone.  pat. 
Immedial  Indone  R cone.  pat. 

6 % 

4 % 

' 1,5% 

307. 

Immedial  Direct  Blue  B pat. 
Immedial  Indone  JBN  cone.  pat. 
Immedial  Indone  R cone.  pat. 

6 % 

308. 

Immedial  Indogene  GCL  cone.  pat. 

6 % 

309. 

Immedial  New  Blue  G cone.  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

7 % 

310. 

Immedial  Direct  Blue  JND  extra 

cone.  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

8 % 

311. 

Immedial  Direct  Blue  BB  extra 

cone.  pat. 

aftertreated  with: 
bluestone  and  bichrome. 

6 % 

312. 

Immedial  Direct  Blue  JB  pat. 
topped  with: 

0,1%  New  Methylene  Blue  N. 

313. 

6 % 

Immedial  Indone  JBN  cone.  pat. 

314. 

6 % 

1 % 

Immedial  Indone  JBN  cone.  pat. 
Immedial  Indone  R cone.  pat. 

315. 

6 % 
1.5% 

Immedial  Indone  JBN  cone.  pat. 
Immedial  Direct  Blue  B pat. 

316. 

5,5% 

Immedial  Direct  Blue  JB  pat. 
topped  with: 

0,1%  New  Methylene  Blue  R. 

317. 

4,5% 

Immedial  Indone  BF  cone.  pat. 

318. 

5 % 

Immedial  Indone  R cone.  pat. 

319. 

7 % 

Immedial  Indone  R cone.  pat. 

320. 

7 % 
2,5% 

Immedial  Indone  JBN  cone.  pat. 
Immedial  Direct  Blue  B pat. 

aftertreated  with: 
bluestone  and  bichrome. 

CASSELLA  COLOR  COMPANY,  NEW  YORK. 

305 


WORKMEN’S  SUITINGS  DYED  WITH  IMMEDIAL  COLOURS, 
DIRECT  AND  AFTERTREATED. 


I! 


313 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


xx 


£ 


BLACK  FOR  LININGS  AND  MOLESKIN. 


321. 

6,5%  Immedial  Black  NN6  cone.  pat. 


322. 

6,5%  Immedial  Brilliant  Black  8BG 

cone.  pat. 


323. 

6,5%  Immedial  Black  BP  cone.  pat. 


324. 

6,5%  Immedial  Brilliant  Black  6BG 

cone.  pat. 


325. 

4,5%  Immedial  Carbon  B pat. 


326. 

4,5%  Immedial  Brilliant  Carbon  FG  pat. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


BLACK  FOR  LININGS  AND  MOLESKIN. 


CASSELLA  COLOR  COMPANY,  NEW  YORK. 


zxi 


_ 


